The Use of Liquid Smoke as a Substitute for Nitric Acid for Extraction of Amorphous silica from Rice husk through Sol-Gel Route
ISSN: 0970-020 X
ORIENTAL JOURNAL OF CHEMISTRY
An International Open Free Access, Peer Reviewed Research Journal
2016, Vol. 32, No. (4): Pg. 2079-2085 www.orientjchem.org
The Use of Liquid Smoke as a Substitute for Nitric Acid
for Extraction of Amorphous silica from Rice husk through
2 WASINTON SIMANJUNTAK *,SIMON SEMBIRING ,
1 KAMISAH, D. PANDIANGAN , FARADILLA SYANI and RUDY, T. M. SITUMEANG 1 Department of Chemistry, the Faculty of Mathematics and Natural Science, 2 The University of Lampung, Indonesia.
Department of Physic, the Faculty of Mathematics and Natural Science, The University of Lampung, Indonesia.
- Corresponding author E-mail: Wasinton.email@example.com http://dx.doi.org/10.13005/ojc/320435
(Received: July 19, 2016; Accepted: August 19, 2016)
ABSTRACTThis study assessed the potential of liquid smoke as substitute for nitric acid for production
of rice husk silica using sol-gel method. The efficacy of liquid smoke was compared to that of 10%
HNO solution in terms of the volume required and the mass of silica obtained. Further evaluation3
was made by comparing the characteristics of the silica as revealed by several characterization
techniques include Fourier infrared spectroscopy, x-ray diffraction, scanning electron microscopy,
and particle size analysis. No significant difference between the volume of the liquid smoke and
the HNO solution required, as well as between the mass of silica obtained. Both samples display3
practically similar functionality and structure. The most interesting finding is that the silica obtained
using liquid smoke exhibits more homogeneous surface morphology and narrower particle size
distribution. Considering its environmentally friendly nature, it was concluded that liquid smoke ismore advantageous than HNO solution. 3 Keywords : Rice husk, silica, sol-gel, liquid smoke.
INTRODUCTION disposed primarily by burning, creating not only air
pollution problems but also the extremely fine silica Rice husk is an agricultural waste abundantly ash, which is also toxic. Furthermore, this treatment available in rice-producing countries, such as practice leads to production of very large amount of
Indonesia. Representing around 20% mass of the CO gas released to the atmosphere and eliminates 1-3 2 whole rice , rice husk is one of the most important the opportunity to utilize the silica free husk for agricultural residues in quantity. Traditionally, rice production of valuables products as value added. husk is considered as a non-valuable waste, and However, rice husk is now considered as valuable
2080 SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016) resource primarily because this agriculture residue has been found to contain 15-20% by mass inorganic components, in which silica is the major constituent with the quantity of 93-99 percent 2 . In recognition of its high silica content, together with availability and renewability considerations, currently rice husk continues to gain growing interest as a potential source of silica. In addition to its high purity, rice husk silica is known as porous and amorphous material 3,4 , which makes it a suitable raw material for production of various silica based materials. Taking advantage of these characteristics, many researchers are currently engaged in exploration of rice husk silica potential, and a wide range of its applications has been reported in literatures, such as production of nanosilica 4,5 , silica gel 6,7 , carbosil 8 , heterogeneous catalysts 9-12 , aluminosilicates 13 , synthetic zeolites 14-16 , and ceramics 17-19 . For production of rice husk silica, two methods have been applied extensively. The first method is thermal extraction by incinerating the husk at 500-1000 o C 20,21 , at which all the organic components are burnt out, leaving the ash containing silica as residue. The second method is commonly known as the sol-gel method. This method involves chemical extraction of silica using alkaline solution such as NaOH 11,22 or KOH 13, 18 , taking advantage of the solubility of the silica in the alkaline solution. The filtrate (silica sol) was then acidified using strong mineral acids, such as HCl 18 , HNO 3 11 or H 2 SO 4 23,24 to bring the sol into neutral condition, at which the silica was transformed from sol into gel state.
Despite their effectiveness, strong acids are relatively expensive and harmful to environment. This is because the water used to wash the gel is finally discharged as corrosive wastewater, causing disposal problem. Considering the environmental hazard together with the price of mineral acids, and in recognition of the growing interest in rice husk silica, this study was carried out to investigate the feasibility of liquid smoke to replace mineral acid for production of silica from rice husk through sol-gel route. To the best of our knowledge, no attempt has been made to use liquid smoke for production of silica powder from rice husk.Utilization of liquid smoke was considered since liquid smoke has sufficient acidity due to the presence of phenols, carbonyls, and organic acids 25,26 , therefore, can be used to neutralize alkaline silica sol, as the case with mineral acids. In addition, liquid smoke is more environmentally friendly agent than strong mineral acids, and can be produced from any biomass by simple pyrolysis treatment. The potential of liquid was evaluated by comparing the amount of liquid smoke with that of HNO 3 solution required, and the characteristics of the silica obtained using both agents.
Experimental methods Materials and instruments
Raw rice husk was obtained from a local rice milling industry. Before use, the husk was soaked in hot water and left overnight. Floating husk was discharged, while sinking husk was collected, rinsed with distilled water, and then oven dried at 110 o C for eight hours. Coconut shell was obtained from a local coconut charcoal industry. Sodium hydroxide and nitric acid used are reagent grade purchased from Merck. The instruments used for characterization of the sample are Varian2000 FTIR spectrometer, an automated Shimadzu XD-610 X-ray diffractometer, a Philips-XL Scanning Electron Microscope, and Particle Size Analyzer, Analysette 22 Nano Tec plus.
Liquid smoke used in this study was prepared in our laboratory (Integrated Laboratory and Center for Technology Innovation, The University of Lampung) by pyrolysis of coconut shell at 450 o
C. Before use, liquid smoke was filtered to remove particulates and applied without further treatment. The liquid smoke was found to have the pH = 1.83.
Rice husk silica was extracted using an alkali extraction process, adopting the method previously applied 11 . Typical experiment was carried out by transferring 50 grams of dry husk into a beaker glass contains 500 mL of 5% NaOH solution. The mixture was boiled for 30 minutes, and then allowed to cool to room temperature and left for 24 hours to optimize the release of silica from the husk. The mixture was filtered to separate the filtrate which contains dissolved silica (silica sol), while the residue was discharged. SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016) 2081 To obtain solid silica, two sol samples with liquid smoke, both samples were characterized equal volume of 200 mL were placed in separate using different techniques. The functionality of the beaker glass. The first sample was neutralized by sample was evaluated using FTIR spectroscopy drop wise addition of 10% HNO solution until the sol carried out on a Perkin Elmer FTIR spectrometer. 3 was completely converted into gel, and the second For measurement, the silica was mixed with solid sample was treated similarly using liquid smoke. The KBr of spectroscopy grade and converted into gels were aged overnight, and then rinsed repeatedly pellet by pressing. To produce FTIR spectrum, the with distilled water to remove the excess of acid or sample was scanned over the wave number range o -1 liquid smoke. The gel was oven dried at 110 C for of 4000-400 cm .Structural evaluation using XRD eight hours, and the mass of solid silica was weighed. technique was conducted using CuKa radiation Solid silica was ground into powder and sieved with ( l = 1.5418 Å), produced at 40 kV and 30 mA, with o 200 mesh sieve, for characterization. a 0.15 receiving slit, recording the pattern over o goniometry (2q) range of 10-40 with a step size of
0.02, using post-diffraction graphite monochromator
To compare the characteristics of silica with a NaI detector. Microstructural analysis was obtained using HNO with that obtained using conducted on polished and thermally-etched sample. 3 Particle size distribution was studied using wet
Table 1: Comparison of sol-gel process to method with distilled water as dispersing solvent.. obtained rice husk silica using HNO and liquid 3 smoke RESULTS AND DISCUSSION Agent Run Volume Mass of Sol-gel process required (mL) silica (gr)
To assess the potential of liquid smoke, the sol-gel process was evaluated in terms of the volume HNO solution
3.92 3 of liquid smoke required as compared to that of HNO 3 (10%)
3.88 solution and the mass of solid silica obtained using
3.91 each agent. For this purpose, sol-gel process using Liquid smoke
3.87 each of the agents was carried out in triplicate, and
3.93 the results obtained are presented in Table 1.
3.96 Fig. 1: The FTIR spectrum of rice husk silica produced using
HNO solution (a), and using liquid smoke (b)
2082 SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016)
Fig. 2: XRD pattern of rice husk silica obtained using nitric acid (a) and using liquid smoke (b)
The experimental data presented in Table 1 clearly indicate that no significant difference between the volume of liquid smoke and HNO 3 solution required and the mass of silica obtained. These findings clearly demonstrated that liquid smoke is comparable to 10%HNO 3 solution, reflecting the potential of liquid smoke to replace mineral acids for sol-gel production of rice husk silica.Further evaluations were based on several characteristics of the silica as described below.
Characteristics of silica
To compare the functionality of the silica obtained using HNO 3 solution and that of silica obtained using liquid smoke, both samples were characterized using FTIR spectroscopy produced the spectra as presented in Figure 1. As can be seen, the spectra are practically very similar, characterized by the existence of several absorption bands associated with rice husk silica commonly reported in literatures 22,24,27-29 . The broad band centered at around 3452 cm
- -1 region is attributed to stretching vibration of hydroxyl (-OH) group of silanol (Si-OH) in the silica and adsorbed water molecules on the surface of the silica. The existence of Si-OH bond is supported by a weak and shoulder band centered at around 980 cm -1
, and the presence of adsorbed water molecules is supported by the absorption band centered at around 1636 cm -1 , which is attributed to bending vibration of the O-H bond. The Si-O-Si bond in the structural framework of the siloxane in the silica is indicated by three characteristic bands, associated with different vibration modes of the bond,
i.e.the band centered at 1082 cm -1
, the band centered at 798 cm
- -1 , and the band centered 457 cm -1
, which are attributed to asymmetric stretching vibration, symmetric stretching vibration, and bending vibration of the Si-O-Si bond, respectively
2083 SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016)
Fig. 4: Particle size distribution of the sample obtained using
nitric acid solution (A) and using liquid smoke (B)
Fig. 3: SEM micrographs of rice husk silica obtained usingHNO 3 solution (a), and using liquid smoke (b)
In the spectra, small peaks were observed at 2996 cm
- -1 represent symmetric and asymmetric
- CH 2 stretching vibrations respectively and at 2355 cm
- -1 represents–CO vibration. The emerge of these organic related functional groups is most likely due to the presence of organic impurities originating from the husk or from the liquid smoke used in the process.
Characterization of the samples using
XRD technique was carried out to evaluate the crystallographic structure of the sample which signifies whether the sample is amorphous or crystalline phase. The XRD patterns of the samples are shown in Figure 2. As generally reported in the literatures 22,30 , the diffraction patterns clearly indicate the existence of the samples as amorphous materials. This amorphous sate of the silica is characterized by the presence of a broad peak centered at 2q = 21.6° (PDF-27-1615).Comparing the patterns it can be observed that the peak for the silica obtained using liquid smoke is broader than that of the silica obtained using HNO 3 solution, suggesting that the sample produced using liquid smoke is more amorphous.
To compare the effect of HNO 3 solution and liquid smoke on microstructures of the samples, both samples were characterized using the technique of SEM, and the surface images produced are shown in
2084 SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016) Figure 3. As can be seen, the two samples displayed significantly different surface morphologies, in which the surface homogeneity of the sample obtained using liquid smoke is significantly higher than that of the sample obtained using nitric acid solution. As can be seen, the surface of the sample obtained using HNO 3 solution is marked by the existence of larger particle sizes and very evident presence of clusters with different sizes, spread all over the surface. The sample obtained using liquid smoke, on the other hand, is characterized by the presence of only a few clusters with considerably smaller sizes than those observed in the sample obtained using nitric acid solution. These different surface characteristics demonstrated that liquid smoke is able to suppress the agglomeration of the silica molecules during the gelation step, thus leading to smaller particle sizes, which is very advantageous in the context of solid material production using sol-gel technique.
3. Shelke, V. R., Bhagade, S. S., and Mandavgane, S. A. Bull.Chem. React. Eng. Catal.2010, 5, 63–67.
9. Adam, F., Kandasamy, K., and Balakrishnan, S. J. Colloid. Interface Sci.2006, 304, 137– 143.
8. Simanjuntak, W., Sembiring, S., and Sebayang, K. Indo. J. Chem.2012, 12, 119-125
7. Rungrodnimitchai, S., Phokhanusai, W., and Sungkhaho, N. J. Met. Mater. Miner.2009, 19, 45-50.
6. Qi, T. and Tao, W. J. Supercrit. Fluids,2005, 35, 91–94.
5. Yuvakkumara, R., Elangoa, V., Rajendrana, V., and Kannanb, N. J. Exp. Nanosci.2014,
4. Amutha, K., Ravibaskar, R. and Sivakumar, G. Int. J. Nano Tech. Appl. 2010, 4, 61-66.
2. Ugheoke, B. I., Mamat, O., andWahjoedi, B.A- .J. Aust. Ceram. Soc.2013, 49, 92 – 100
For further evaluation of the particle size profile, both samples were characterized using PSA technique, and the results obtained are shown in Figure 4.
Tech.2012, 2, 210-213.
REFERENCES1. Olamide , O. and Oyawale, F. A. Int. J. Sci.
The authors gratefully acknowledge The Directorate of Higher Education, The Ministry of Research, Technology, and Higher Education, Republic of Indonesia, for financial support through research grant, Hibah Kompotensi 2016, contract number: 78/UN26/8/LPPM/2016.
The results of this study demonstrated the efficacy of liquid smoke as substitute for mineral acids for production of rice husk silica using sol-gel technique. The volume of liquid smoke required and the mass of silica obtained are comparable to those of 10% HNO 3 solution. The most interesting results are more homogeneous surface morphology and narrower particle size distribution of the silica obtained using liquid smoke than those of the silica produced using HNO 3 solution. These different surface characteristics demonstrated that liquid smoke is able to suppress the agglomeration of the silica molecules during the gelation step, which is very advantageous in the context of solid material production using sol-gel technique. Considering the performance and environmentally friendly nature of liquid smoke, it is then concluded that utilization of liquid smoke for production of rice husk silica is more advantageous than HNO 3 solution, and more likely than other mineral acids.
As can be seen, the particle size distributions of the samples are significantly different, in which very evident smaller particle sizes and narrower range of the particle distribution is displayed by the sample obtained using liquid smoke. The sample obtained using nitric acid solution has the size in the range of 1142 – 3712 nm, while that obtained using liquid smoke has the particle size in the range of 194 - 680nm. It should be noted that the particle size distributions of two samples are not perfectly symmetric, which most likely due to the presence of aggregates as evidently revealed by the SEM results in Figure 3.
10. Ahmed, A. E. and Adam, F. Micropor.
2085 SIMANJUNTAK et al., Orient. J. Chem., Vol. 32(4), 2079-2085 (2016) 11. Pandiangan, K. D. and Simanjuntak, W. Indo.
22. Yuvakkumara, R., Elangoa, V., Rajendrana, V., and Kannanb, N. J. Exp. Nanosci.2014, 9, 272 –281.
46 30. Edson, L. F. and Ederson, G. J. Mat. Sci.
29. Abadi, M. H. S., Delbari, A., Fakoor, Z., and Baedi, J. J. Ceram. Sci. Tech. 2015, 06, 41-
E. P. Int. J.Sci. Environ.Technol.2013, 2, 1027–1035.
28. Dominic , M. C. D., Begum, S. P. M., Joseph, R., Joseph, D., Kumar, P. and Ayswarya
27. Guo Y., Wang M., Zhang H., Liu G., Zhang L. and Qu X.J. Appl. Polym. Sci.2008, 107, 2671-2680.
26. Wititsiri, S. J. Sci. Technol. 2011, 33, 349- 354.
D., and Anklam, E. J. Sep. Sci. 2005, 28, 871–882.
25. Simon, R., de la Calle, B., Palme, S., Meier,
Chem. Soc. Pak. 2014, 36, 382-387.
24. Ul Haq, I., Akhtar, K., and Abdul Malik, A. J.
J. Electrochem. Sci. 2013, 8,1759 – 1769.
23. Awizar, D. A., Othman, N. K., Jalar, A., Daud, A. R., Rahman, I. A., and Al-hardan, I. N. Int.
21. Rafiee, E., Shahebrahimi, S., Feyzi, M. and Shaterzadeh, M. Int. Nano Let.2012, 12, 1-8.
J. Chem. 2013, 13, 47-52.
20. Rozainee, M., Ngo, S. P., Arshad, A. S. and Tan, K. G. Energy Sustain.Dev.2008, 12, 33–42.
Int.2016, 14, 8431-8437
19. Sembiring, S., Simanjuntak, W., Situmeang, R., Riyanto, A., and Kerista, S. Ceram.
18. Sembiring, S., Simanjuntak, W., Manurung, P., Asmi, D., and Low, I. M. Ceram. Int.2014, 40, 7067–7072.
17. Sembiring, S. (2011). Indo. J. Chem. 2011, 11, 85 – 89.
16. Ali, I. O., Hassan, A. M., Shaaban, S. M., and Soliman, K. S.Sep. Purif. Technol. 2011, 83, 38–44.
15. Rahman, M. M., Hasnida, N., and Wan Nik, W. B.J. Sci. Res. 2009, 1, 285-291.
V. K-.Micropor. Mesopor. Mat.2008, 115, 189- 196.
14. Kardatos, K., Gavela, S., Ntziouni, A., Pistiolas, K. N., Krytsi, A., and Rigopoulou,
, 39, 9369–9375
13. Simanjuntak, W., Sembiring, S., Manurung, P., Situmeang, R., and Low, I. M. Ceram. Int.
12. Pandiangan, K. D., Jamarun, N., Arief, S., and Simanjuntak, W. Orient. J. Chem.2016, 32, 385-390.
Tech.2006, 9, 206-215.